- Nano Express
- Open Access
Temperature Dependence of Raman-Active In-Plane E2g Phonons in Layered Graphene and h-BN Flakes
Nanoscale Research Letters volume 13, Article number: 25 (2018)
Thermal properties of sp2 systems such as graphene and hexagonal boron nitride (h-BN) have attracted significant attention because of both systems being excellent thermal conductors. This research reports micro-Raman measurements on the in-plane E2g optical phonon peaks (~ 1580 cm−1 in graphene layers and ~ 1362 cm−1 in h-BN layers) as a function of temperature from − 194 to 200 °C. The h-BN flakes show higher sensitivity to temperature-dependent frequency shifts and broadenings than graphene flakes. Moreover, the thermal effect in the c direction on phonon frequency in h-BN layers is more sensitive than that in graphene layers but on phonon broadening in h-BN layers is similar as that in graphene layers. These results are very useful to understand the thermal properties and related physical mechanisms in h-BN and graphene flakes for applications of thermal devices.
Both graphene and hexagonal boron nitride (h-BN) flakes have a layered structure, with weak Van der Waals (vdW) interactions keeping the layers together but strong sp2 chemical bonds making atoms held together within each layer [1, 2]. Due to the layered structure, these two materials are excellent thermal conductors [3, 4] and their thermal properties have attracted significant attention [5, 6]. The thermal transports in them are dominated by lattice vibrations and are described properly by phonon scattering [7,8,9]. There is a Raman-active mode with symmetry E2g describing in-plane atoms movement, which is named as G peak [10, 11] in graphene layers and E2ghigh peak [12, 13] in h-BN layers (distinguishes from the low frequency E2g mode at about 53 cm−1 [14, 15], denoted as E2glow). The frequency shifts and broadenings of these two-phonon scattering peaks are dependent on the elongation of the intra-layer C–C bond (or B–N bond) and meanwhile the number of layers [16, 17] due to thermal expansion or multi-phonon anharmonic couplings [9, 18, 19]. Thus, the in-plane E2g phonon plays an important role in the study of thermal properties of sp2 materials. Several papers have reported the temperature dependence of the frequency or linewidth of G peak or E2ghigh peak in the Raman spectra of ultrathin graphene layers [9, 16, 17], bulk graphite [9, 18], and bulk h-BN [14, 19], respectively. However, the temperature effect on in-plane E2g phonon in graphene as well as h-BN layers and the thermal properties of these two materials still lack of a detailed comparison.
In this research, we measured G peak in graphene layers and E2ghigh peak in h-BN layers by micro-Raman spectroscopy at the temperature range from − 194 to 200 °C. Temperature dependence of frequency shifts and broadenings of these two peaks were investigated in graphene and h-BN layers with similar thickness. Furthermore, the thermal effect in the c direction on their frequency shifts and broadenings was studied in graphene and h-BN layers as thickness increases. A similar comparison has not yet been reported previously. Therefore, Raman microscopy is a very useful tool to investigate the thermal properties for micro-scale flakes of graphene- and h-BN-layered structures.
Graphene flakes and h-BN flakes were obtained by micromechanical cleavage of bulk graphite crystals and bulk single-crystalline BN platelet on SiO2/Si substrate with SiO2 thickness as 90 nm. Layered graphenes and h-BNs can be easily seen under a microscope. We selected some flakes with dozens of atomic layers to avoid the higher influence of adsorbates and charge transfer from SiO2/Si substrate  and to eliminate the heating enhancement in ultrathin graphene and h-BN layers. The thickness of graphene flakes and h-BN flakes was determined by atomic force microscopy (AFM) measurement with a tapping mode. Figure 1 shows the microscope images of four selected h-BN and graphene flakes, and their AFM images as well as the thickness measured in the black rectangles highlighted in microscope images. Figure 1a, b shows two h-BN flakes with the thickness of 16.2 and 36.2 nm, and Fig. 1c, d shows two graphene flakes with the thickness of 16.5 and 35.6 nm, respectively. They are selected to have similar thickness in order to facilitate the comparison for temperature dependence of frequency shifts and broadenings of phonons in micro-Raman spectroscopy.
The temperature-dependent Raman spectra of G peak and E2ghigh peak were measured in back-scattering with a HR Evolution micro-Raman system, equipped with the unique SWIFT™ CCD, a × 50 objective lens (NA = 0.45). The samples were mounted on an in-house-made sample holder consisting of a thin copper disk with a central pillar and a 500-μm diameter hole. Measurements from − 194 °C to 200 °C were carried out in a liquid nitrogen (LN2) cooled low-temperature Linkam stage equipped with a temperature controller. All spectra were excited with a 532-nm laser and recorded with an 1800 lines/mm grating to enable each pixel of the charge-coupled detector to cover 0.5 cm−1. A laser power below 2 mW was used to avoid sample heating. The integration time of 20 s was adopted to ensure a good signal-to-noise ratio.
Results and Discussion
The G peak and E2ghigh peak are representative in-plane Raman modes. We first illustrated Raman spectra of the four selected flakes (shown in Fig. 1) at room temperature in Fig. 2, in which the curves from bottom to top are given in the order of increasing thickness and the curves are offset for clarity. Figure 2a shows Raman spectra of h-BN flakes in the spectral range from 100 to 1800 cm−1. The peaks at about 300, 520, and 940 cm−1 are characteristic peaks of Si substrate , and the E2ghigh peak is at about 1362 cm−1. The frequency of the E2ghigh peak is almost the same in two flakes. Yet the Si peaks at the 36.2 nm h-BN flake are weaker than that at the 16.2 nm h-BN flake due to more absorption of Raman signals in a thicker flake . Figure 2b shows Raman spectra of graphene flakes in the spectral range from 100 to 3000 cm−1, which consists of the Si peaks of Si substrate, G and 2D peaks of graphene flakes. The positions of Si peaks are the same with those in Fig. 2a. G peak appears around 1580 cm−1, and 2D peak is at around 2700 cm−1 which is a second-order Raman mode and is another fingerprint of graphene layers . The G peak exhibits no significant difference in frequency, while the intensities of Si peaks decrease as the thickness of graphenes increases. G peaks are much stronger than E2ghigh peaks because resonant excitation is easy to be satisfied in graphene layers due to its zero gap . The second-order Raman peaks of h-BN layers have not been obtained for the reason that Raman processes are non-resonant in h-BN layers when laser source is in the visible range . There are no defective Raman peaks in h-BN and graphene layers, meaning that these flakes are defect-free crystals, which are suitable prototype systems to study the temperature dependence of in-plane E2g phonons.
We further measured variable temperature Raman spectra of G peak or E2ghigh peak on chosen four flakes in the temperature range of − 194~200 °C, as shown in Fig. 3. It is obvious that both G peaks and E2ghigh peaks show a progressive downshift as the temperature increases. The Raman peaks were fitted by a single Lorentzian profile to obtain their frequencies and full width at half maximum (FWHMs).
Figure 4a shows the frequency shifts of G peak and E2ghigh peak. In theory, the temperature dependence of phonon pulsation ωph in both E2ghigh peak and G peak indicates a nonlinear relationship, which can be described by fitting a second-order polynomial, ωph = ωph0 + at+bt2 [18, 19]. Here, ωph0 is the phonon frequency at 0 °C. The thermal frequency shifts are best fitted, and the constants of ωph0, a, and b are given in Table 1. We obtained some results from these constants.
First, ωph0 in two h-BN flakes is the same as 1363 cm−1 and in two graphene flakes is the same as 1579 cm− 1. It means that frequencies of both two E2g modes are independent on thickness at about 0 °C. Their frequency differences at 25 °C are below 0.5 cm− 1 with different thickness, which is below the resolution of the Raman system. This is why the E2ghigh peak and G peak positions show no shifting in different thickness at room temperature in Fig. 2. Second, with increasing temperature, E2ghigh and G modes display a marked frequency downshift. The shifts of the E2ghigh peak are − 18 and − 12 cm− 1 in 16.2 and 36.2 nm h-BN flakes respectively in the temperature from − 194 to 200 °C, whereas the shifts of G peak in two graphene flakes are smaller and remain below − 10 cm−1. This shows that the frequency shift of E2ghigh peak is about 1.4–2.1 times than that of G peak in the similar thickness of h-BN and graphene flakes as the temperature varied by Δt ~ 400 °C. Our experimental results can find some supporting evidence from previous calculation results. In the reference  and , frequency shifts of E2g phonon are calculated in bulk h-BN  and bulk graphite  by three-phonon, four-phonon, and thermal expansion contributions. The frequency shift of E2ghigh peak in bulk h-BN from 100 to 600 K is about − 10 cm−1 , but that of G peak in bulk graphite from 100 to 600 K is about − 5 cm−1 . We can see that multi-phonon coupling plays a major role on frequency shifts. Thus, h-BN flakes show higher sensitivity to temperature-dependent frequency shifts than graphene flakes, which should be attributed to stronger multi-phonon coupling in h-BN flakes.
Figure 4b shows the FWHMs of G peak and E2ghigh peak. In the temperature range of interest here, the linewidth of both modes indicates a linear relationship. Similar behavior has been reported for bulk h-BN with temperature below 400 K . We fitted the relation between temperature and FWHM by a first-order polynomial, Γph = Γph0 + ct, where Γph0 is the FWHM at 0 °C. The constants of Γph0 and c are given in Table 2. Some results can be seen from these constants.
The FWHM of the E2ghigh peak is 7 ~ 10 cm−1 in two h-BN flakes, whereas the FWHM of G peak in two graphene flakes is larger and remains 13 ~ 14 cm−1. They are in good agreement with the experimental results reported in bulk graphite  and bulk h-BN . The E2ghigh modes exhibit a sizable broadening of ~ 1 cm−1 as temperature increases; in contrast, G modes show an insignificant broadening in the temperature range studied. It means that the lifetime of the E2ghigh peak is more sensitive to the temperature variation than that of G peak in the similar thickness of h-BN and graphene flakes as the temperature varied by Δt ~ 400 °C. Our experimental results can be explained in terms of the calculation of the references  and . The FWHM broadenings of E2g phonon are calculated in bulk h-BN  and bulk graphite  by three-phonon and four-phonon contributions. The FWHM broadening of the E2ghigh peak in bulk h-BN from 100 to 300 K is about 1.5 cm−1 , but that of G peak in bulk graphite from 100 to 300 K is about zero . The multi-phonon coupling also plays a major role on FWHM broadenings. Thus, h-BN flakes show higher sensitivity to temperature-dependent FWHM broadenings than graphene flakes, which we think should be also attributed to stronger multi-phonon coupling in h-BN flakes.
In addition, with increasing thickness, the frequency shifts of both G peak and E2ghigh peak become smaller. It is in good agreement with the experimental results reported in references [16, 17], in which Calizo el al. found that the shift of G peak in bilayer graphenes is larger than those in graphite as the temperature varied from 100 to 400 K , and the shift of G peak in monolayer graphenes is larger than that in bilayer graphenes as the temperature varied from − 200 to 100 °C . In this paper, the frequency shifts related to the c direction thickness are evaluated to be − 8.9 × 10−4 cm−1/(°C nm) in h-BN layers and − 3.5 × 10−4 cm−1/(°C nm) in graphene layers, respectively, in the temperature range from − 194 to 200 °C. The frequency shift in the c direction of the E2ghigh peak is ~ 2.5 times that of G peak as the temperature varied by Δt~400 °C. Meanwhile, the slopes of the FWHM of both G peak and E2ghigh peak have a slight increase with increasing thickness. The FWHM broadenings related to the c direction thickness are evaluated to be 5.5 × 10−5 cm− 1/(°C nm) in h-BN layers and 5.9 × 10−5 cm−1/(°C nm) in graphene layers, respectively, in the temperature range from − 194 to 200 °C. The FWHM broadening in the c direction of the E2ghigh peak has the same sensitivity to temperature as that of G peak. This means that the thermal effect in the c direction on phonon frequency in h-BN layers is more sensitive than that in graphene layers but on phonon broadening in h-BN layers is similar as that in graphene layers. However, we can hardly find relevant theoretical calculations about the frequency shift and the FWHM broadening of E2g phonons with increasing h-BN or graphene thickness to explain the physical mechanism of our experiment. We think our results are attributed to joint contributions of anharmonic interaction and other more complex couplings. The mechanisms are still not well understood and need further study.
Graphene and h-BN layers are isoelectronic materials. Their in-plane sp2 structures exhibit a similar hexagonal structure with similar lattice parameters, and they are usually stacked to form a multilayer in a stable configuration of AB stacking when prepared by mechanical exfoliation. Given the similarities of an atom structure, the properties of these two materials are expected to be similar to facilitate the comparison. Raman spectroscopy is a powerful characterization tool for graphene and h-BN materials with respect to thermometry. We performed a Raman scattering study of in-plane E2g phonons in layered h-BN and graphene flakes in the temperature range from − 194 to 200 °C. The frequency shifts and FWHM broadenings of E2ghigh peak and G peak indicate that h-BN flakes are more sensitive to temperature than graphene flakes with similar thickness. The effect of the thermal conduction in the c direction on phonon frequency in h-BN layers is better than that in graphene layers but on phonon broadening in h-BN layers is similar as that in graphene layers. These results are very useful to further understand the thermal properties and related physical mechanisms in h-BN and graphene flakes for applications of thermal devices.
Atomic force microscopy
Full width at half maximum
Hexagonal boron nitride
Van der Waals
Marom N, Bernstein J, Garel J, Tkatchenko A, Joselevich E, Kronik L et al (2010) Stacking and registry effects in layered materials: the case of hexagonal boron nitride. Phys Rev Lett 105:046801
Partoens B, Peeters FM (2006) From graphene to graphite: electronic structure around the K point. Phys Rev B 74:075404
Seol JH, Jo I, Moore AL, Lindsay L, Aitken ZH, Pettes MT et al (2010) Two-dimensional phonon transport in supported graphene. Science 328:213
Zheng JC, Zhang L, Kretinin AV, Morozov SV, Wang YB, Wang T et al (2016) High thermal conductivity of hexagonal boron nitride laminates. 2D Mater 3:011004
Balandin AA, Ghosh S, Bao WZ, Calizo I, Teweldebrhan D, Miao F et al (2008) Superior thermal conductivity of single-layer graphene. Nano Lett 8:902
Wang CR, Guo J, Dong L, Aiyiti A, Xu XF, Li BW (2016) Superior thermal conductivity in suspended bilayer hexagonal boron nitride. Sci Rep 6:25334
Menendez J, Cardona M (1984) Temperature dependence of the first-order Raman scattering by phonons in Si, Ge, and a-Sn: anharmonic effects. Phys Rev B 29:2051
Su LQ, Zhang Y (2015) Temperature coefficients of phonon frequencies and thermal conductivity in thin black phosphorus layers. Appl Phys Lett 107:071905
Bonini N, Lazzeri M, Marzari N, Mauri F (2007) Phonon anharmonicities in graphite and graphene. Phys Rev Lett 99:176802
Ferrari AC, Basko DM (2013) Raman spectroscopy as a versatile tool for studying the properties of graphene. Nat Nanotechnol 8:235
Ferrari AC, Meyer JC, Scardaci V, Casiraghi C, Lazzeri M, Mauri F et al (2006) Raman spectrum of graphene and graphene layers. Phys Rev Lett 97:187401
Reich S, Ferrari AC, Arenal R, Loiseau A, Bello I, Robertson J (2005) Resonant Raman scattering in cubic and hexagonal boron nitride. Phys Rev B 71:205201
Geick R, Perry CH, Rupprecht G (1966) Normal modes in hexagonal boron nitride. Phys Rev 146:543
Stenger I, Schue L, Boukhicha M, Berini B, Placais B, Loiseau A et al (2017) Low frequency Raman spectroscopy of few-atomic-layer thick hBN crystals. 2D Mater 4:031003
Kuzuba T, Era K, Ishii T, Sato T (1978) A low frequency Raman-active vibration of hexagonal boron nitride. Solid State Commun 25:863
Calizo I, Miao F, Bao W, Lau CN, Balandin AA (2007) Variable temperature Raman microscopy as a nanometrology tool for graphene layers and graphene-based devices. Appl Phys Lett 91:071913
Calizo I, Balandin AA, Bao W, Miao F, Lau CN (2007) Temperature dependence of the Raman spectra of graphene and graphene multilayers. Nano Lett 7:2645
Giura P, Bonini N, Creff G, Brubach JB, Roy P, Lazzeri M (2012) Temperature evolution of infrared-and Raman-active phonons in graphite. Phys Rev B 86:121404(R)
Cusco R, Gil B, Cassabois G, Artus L (2016) Temperature dependence of Raman-active phonons and anharmonic interactions in layered hexagonal BN. Phys Rev B 94:155435
Mishra P, Jain KP (2001) First- and second-order Raman scattering in nanocrystalline silicon. Phys Rev B 64:073304
Li XL, Qiao XF, Han WP, Lu Y, Tan QH, Liu XL, Tan PH (2015) Layer number identification of intrinsic and defective multilayered graphenes up to 100 layers by the Raman mode intensity from substrates. Nano 7:8135
Geim AK, Novoselov KS (2007) The rise of graphene. Nat Mater 6:183
Watanabe K, Taniguchi T, Kanda H (2004) Direct-bandgap properties and evidence for ultraviolet lasing of hexagonal boron nitride single crystal. Nat Mater 3:404
This research is supported by the Youth Project of the National Natural Science Foundation of China (11504077), the National Natural Science Foundation of China (61774053), the Youth Project of Hebei Province Natural Science Foundation (A2017201012), and the Key Project of Hebei Province Department of Education Fund (ZD2017007).
Availability of Data and Materials
Graphene flakes and h-BN flakes were obtained by micromechanical cleavage of bulk graphite crystals (2D semiconductors Inc.) and bulk single-crystalline BN platelet (2D semiconductors Inc.) on SiO2/Si substrate with SiO2 thickness as 90 nm. The Raman spectra were measured in back-scattering with a HR Evolution micro-Raman system, equipped with the unique SWIFT™ CCD, a × 50 objective lens (NA = 0.45). Measurements from − 194 to 200 °C were carried out in a liquid nitrogen (LN2) cooled low-temperature Linkam stage equipped with a temperature controller.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Li, X., Liu, J., Ding, K. et al. Temperature Dependence of Raman-Active In-Plane E2g Phonons in Layered Graphene and h-BN Flakes. Nanoscale Res Lett 13, 25 (2018). https://doi.org/10.1186/s11671-018-2444-2
- In-plane E2g phonon
- Temperature dependence